Slideshare uses cookies to improve functionality and performance, and to provide you with relevant advertising. If you continue browsing the site, you agree to the use of cookies on this website. See our User Agreement and Privacy Policy.

Slideshare uses cookies to improve functionality and performance, and to provide you with relevant advertising. If you continue browsing the site, you agree to the use of cookies on this website. See our Privacy Policy and User Agreement for details.

Like this document? Why not share!

2,080 views

1,993 views

1,993 views

Published on

Steel structures by Vesrgese

No Downloads

Total views

2,080

On SlideShare

0

From Embeds

0

Number of Embeds

3

Shares

0

Downloads

95

Comments

0

Likes

1

No embeds

No notes for slide

- 1. CHAPTER 17Fatigue-resistant DesignIntroductionThe word ‘fatigue’ originated from the Latin expression ‘fatigare’ which means‘to tire’. The term fatigue was coined by Braithwaite in 1854. Fatigue is the initiationand propagation of microscopic cracks into macro cracks by the repeated applicationof stress(es) (Lu & Mäkeläinen 2003). The damage and/or failure of materialsunder cyclic loads in engineering applications is called fatigue damage. Fatiguefailures generally take place at a stress much lower than the ultimate strength (yieldstress) of the material—at a stress which is considered safe on the basis of staticfailure analysis. The failure is due primarily to the repeated stress from a maximumto a minimum. Fatigue failure may occur in many different forms: mechanicalfatigue, when the components are under only fluctuating stress or strain; creepfatigue, when the components are under cyclic loading at high temperature; thermo-mechanical fatigue, when both mechanical loading and temperature are cyclic;corrosion fatigue, when the components are under cyclic loading in the presenceof a chemically aggressive environment (Ramachandra Murthy 1994; RamachandraMurthy et al. 1994). The major loads that a building is subjected to are dead, live, wind, andearthquake loads. Dead and live loads are always present. However, the designlive loads may be experienced by the structure only once or twice a year. Theoccurrence of the design wind and seismic loads, which are cyclic in nature, willbe about 1 in 50 years. The occurrence of cyclic stresses in buildings is usuallycaused by machinery and the induced cyclic stresses are typically low. Steel canwithstand an infinite number of load reversals at low stresses. Hence, in buildings,fatigue is not considered in the design of members. Examples of structures whichare prone to fatigue are bridges, gantry girders, cranes, slender tower-like (open)structures (subject to wind oscillations), offshore platforms (subject to wave load),and structures supporting large rotating equipment. For these structures, verificationsin the limit state of fatigue are often more critical than in the serviceability orultimate limit state. This implies that the fatigue resistance for these structures maybe more critical than structural stiffness or strength. Fatigue cracking has been the single largest cause of the damage requiring repair(forming 31.3% of the total damage) to the offshore platforms in the North Sea
- 2. 17.2 Design of Steel Structures(Ramachandra Murthy 1998). The primary reason for the collapse of theaccommodation platform ‘Alexander L. Kielland’ in the year 1980 in the NorthSea, which killed 212 men on board, was the failure of a brace due to fatiguecracking. More than 75% failures in steel structures, especially in welds or weldedstructures, are attributed directly or indirectly due to fatigue cracking (RamachandraMurthy & Seetharaman 1997). Fatigue failure is progressive in nature and involves the following four stages:(1) crack initiation at the points of concentrated stress, (2) crack growth, (3) crackpropagation, and (4) final rupture. The failure begins with a slip in the crystallinestructure of the metal followed by the development of microscopic cracks, whichgradually increase in size in a slow and steady mode. (Crack initiation alwaysoccurs in points of flaw in the material or stress concentrations.) This progressivecracking usually results in ‘striation’ marks (also called clam shell or oyster shellmarks), which are concentric rings that point toward the area of the initiation(Gaylord et al. 1992; Lu & Mäkeläinen 2003). The cracked surface with striationsis a clear indication of the fatigue crack (see Fig. 17.1). Although somewhat similarin appearance, striations are not beach marks as one beach mark may containthousands of striations. The extent of the fatigue crack gradually increases withthe subsequent load repetitions. The fracture line will not be easily visible on thesurface of the member in service conditions but can be detected with non-destructivetesting techniques. The final (catastrophic) failure generally occurs in regions oftensile stress when the reduced cross section becomes insufficient to carry thepeak load without rupture. Fatigue damage of structures subject to elastic stressfluctuations occurs at regions where the localized stress exceeds the yield stress ofthe material. After a certain number of load fluctuations, the accumulated damagecauses the initiation and subsequent propagation of crack(s) in the plasticallydamaged regions. This process can cause the components fracture. The usualappearance of the face of fatigue fracture is shown in Fig. 17.2 (Clarke & Coverman Fig. 17.1 Typical striations around an inclusion (Lu & Mäkeläinen 2003)
- 3. Fatigue-resistant Design 17.3 Fig. 17.2 Appearance of fatigue fracture surface (Clarke & Coverman 1987)1987). Another possible mode of failure is that the fracture limit state is reached(brittle fracture) after a fatigue area has grown to a critical size (Kulak & Gilmor1998). The large final fracture area for a given material indicates a high maximumload, whereas a small area indicates a low fracture load (Lu & Mäkeläinen 2003). Fatigue failures may be classified as high-cycle and low-cycle fatigue failures.Under high-cycle fatigue, the material deforms primarily elastically, and the numberof cycles for failure, or the failure time, is characterized in terms of the stressrange. Low-cycle fatigue can be characterized by the presence of macroscopiccyclic plastic strains as evidenced by a stress–strain hysteresis loop. Depending onthe material strength and ductility, the upper limit of the low-cycle fatigue regimemay be from 100 to 100,000 cycles or more. For common ductile structural materials,the low-cycle fatigue regime is generally limited to less than 50,000 cycles.Source of FlawsAs already discussed, the crack initiation is due to the effect of stress concentrationsor flaw(s) in the material. Stress concentrations arise due to sudden changes in thegeneral geometry (e.g., ‘notch’ intersection of two elements) of a member andfrom local changes due to bolt and rivet holes. Stress concentration also occurs atdefects in the member or its connectors and welds. These may be due to the originalrolling of steel or subsequent fabrication such as poorly made welds, rough edgesresulting from shearing, punching, or flame cutting. Flaws in rolled shapes arise from surface and edge imperfection: irregularitiesin mill scale, laminations, seams, inclusions, etc. due to material handling, cutting,shearing, etc. (Ramachandra Murthy & Seetharaman 1997). Punched holes give a greater reduction in fatigue life than drilled and reamedholes because of the imperfections at the hole edges arising from the punchingprocess. In any case, the crack starts at the edge of the hole. Such flaws may not benoticed during fabrication or erection but, as discussed already, they give rise tocracks under cyclic loading.
- 4. 17.4 Design of Steel StructuresDefects in Welded MembersIn welded steel structures most of the fatigue cracks start to grow from welds,rather than from other details, because of the following points (Gurney 1979; Fisher1984; Maddox 2005). 1. Most welding processes leave minute metallurgical discontinuities, from which cracks may grow. As a result, the initiation period needed to start a crack in the material is either very short or not existent. Cracks, therefore, spend most of their life propagating, i.e., getting longer. 2. Most structural welds have a rough profile. Sharp changes in direction generally occur at the toes of butt welds and at the toes and roots of fillet welds (see Fig. 17.3). These points cause local stress concentrations (see Fig. 17.4). Small discontinuities close to these points will therefore react as though they are in a more highly stressed member and grow faster. Fig. 17.3 Local stress concentration at welds Fig. 17.4 Typical stress distribution at weld toe
- 5. Fatigue-resistant Design 17.5 Imperfection in welds include the following (Gurney 1979; Barsom & Rolfe1999): l Volumetric (blow holes and pores and slag inclusion) imperfections l Planer imperfections (cracks and lack of fusion) l Imperfections introduced due to the weld geometry (weld reinforcement, inclusion around a weld repair or at start–stop locations or at arc strikes and undercut) l Imperfection of the weld geometry (angular and axial misalignment)Some of these imperfections are shown in Fig. 17.5. Fig. 17.5 Imperfections in welds Imperfections lower the fatigue strength and are caused by the followingprocesses (Barsom and Rolfe 1999): l Improper design that restricts accessibility for welding l Improper choice of the electrode and flux l Incorrect selection of the welding process l Human errors such as welder’s negligence Although the fabricator of the structure and the weld inspector (who certifiesthe quality of welds) may try to minimize these defects, it is neither practical noreconomically feasible to eliminate all these imperfections. Thus, the potential forfatigue crack growth exists in every steel structure subjected to alternating loads.Also, the initiation phase of fatigue crack growth does not exist in most weldedstructures, since the crack is available already in the form of an existing flaw ordiscontinuity. However, fortunately the crack growth requires a relatively largenumber of cycles of loading. As discussed in Chapter 2, the fracture due to fatigue is an ultimate (safety)limit state and the fatigue strength is always checked under service-load conditions.Hence the task of the structural engineer is to proportion the structural members(that have the potential for failure by fatigue crack growth) such that they will havelong life compared to the design life of the structure.17.1 Factors Affecting Fatigue LifeOf the many factors that affect the fatigue life, the following three factors arefound to be very important. 1. The number of cycles of loading to which the member is subjected to. 2. The stress range at the location (the algebraic difference between the maximum nominal stress and the minimum nominal stress. The nominal stresses are those
- 6. 17.6 Design of Steel Structures determined from the applied loading and using the cross-sectional properties of the members using the basic theory of the strength of materials). 3. The type of member/detail at the location.The other factors that influence the fatigue behaviour are (a) stress concentration,(b) residual stress in the steel, (c) plate thickness, (d) material strength,(e) imperfections, (f ) stress ratio, (g) frequency of cyclic loading, (h) post-weldtreatment, (i) service temperature of the steel, and ( j) environment (important inthe case of corrosion fatigue). Some of these factors are discussed briefly in thefollowing.Stress concentration Fatigue failure is often enhanced by the stress concentrationat the tip of flaws such as holes, notches, etc. as shown in Fig. 17.6. Notchescannot be avoided in structures and machines. A bolt has notches in thread rootsand at the transition between the head and the shank. The stress at these points willbe more than three times the average applied stress. When the load is cyclic, thestress fluctuates between tension and compression and points m and n (see Fig. 17.6)experience a higher range of stress reversal than the applied average stress. Due tothe fluctuations involving higher stress ranges, minute cracks appear at these points(Fig. 17.7). The final fracture occurs when the crack length reaches a critical value Fig. 17.6 Stress concentrations in the presence of notches and holes Fig. 17.7 Fatigue cracks at holes and notches
- 7. Fatigue-resistant Design 17.7ae or the stress intensity factor KI reaches the critical value KIC (which is termed asfracture toughness). The fracture toughness can be determined experimentally from tests with apredetermined crack of length a. KIC assumes the fracture without plasticdeformation. For relatively thin plates, larger plastic deformations occur and thecritical intensity factor is then defined as KC, which is higher than KIC. Any abrupt discontinuity or change in the section of a member, such as a sharpre-entrant corner, interrupts the transmission of stress along smooth lines (seeFig. 17.8). The magnitude of the stress concentration increases as the abruptnessof the discontinuity increases (Lu & Mäkeläinen 2003). These localizedconcentrations, including those at the toe of longitudinal welds, have significanteffect on fatigue strength. Fig. 17.8 Stress flow at re-entrant cornersResidual stresses As discussed in Chapter 1, residual stresses are those that existin a component that is free from externally applied loads. They are caused by non-uniform plastic deformations in neighbouring regions. Furthermore, residual stressesare always balanced so that the stress field is in static equilibrium. Because thefatigue life is governed by the stress range instead of stresses, tensile residualstresses usually have only a secondary effect on the fatigue behaviour ofcomponents. On the other hand, excessive tensile residual stress can also initiatean unstable fracture in materials with a low-fracture toughness. The effect ofcompressive residual stress may increase the fatigue resistance for a lower level ofstress. In welded components, residual stresses are caused by the inability of thedeposited molten weld metal to shrink freely as it cools and solidifies. The magnitudeof the residual stresses depends on such factors as the deposited weld beads, weldsequence, total volume of deposited weld metal, weld geometry, and the strengthof the deposited weld metal with respect to the adjoining base metal. Often themagnitude of these stresses exceeds the elastic limit of the lowest strength regionin the weldment (Barsom & Rolfe 1999).Plate thickness The thickness of the plate has an adverse effect on the fatiguestrength due to the following reasons (Fricke 2003).Stress gradient effect The tensile region of the stress field (including residualstresses) around the weld toe is larger in thicker plates so that an initial defectexperiences a larger stress during crack initiation and early crack propagation,thus resulting in a shorter fatigue life.
- 8. 17.8 Design of Steel StructuresTechnological size effect This effect is mainly attributed to the material size andsurface effects. In particular, for welded joints, the ratio between the plate thicknessand the weld toe radius is larger for thicker plates, resulting in a higher stressconcentration and, hence, in a reduced crack initiation period.Statistical size effect The likelihood of finding a significant defect in a larger volumeis increased compared to a smaller one.Material strength The grade of steel has no apparent effect on the number ofcycles to failure. In general, the fatigue resistance of steel is proportional to itsultimate strength. Under ideal conditions, the fatigue limit is approximately 35%–50% of the ultimate tensile strength for most steels and copper alloys. The generalrelation between the fatigue limit ( fl) and the ultimate stress ( fu) is given by(Ramachandra Murthy 1998) fl = 140 + 0.25fu (in MPa) (17.1)Imperfections Normally the imperfections and flaws discussed in the previoussections can cause stress concentration that lowers the fatigue strength. The severityof a discontinuity, which is due to imperfections, is governed by its size, shape,and orientation, as well as the magnitude and direction of the design and fabricationstresses. Generally, the severity of discontinuity increases as the size increases andas the geometry becomes more planar and the orientation more perpendicular tothe direction of tensile stresses. Thus volumetric discontinuities are usually lessinjurious than planar, crack-like discontinuities. Also the crack-like discontinuitieswhose orientation is perpendicular to the tensile stress can be injurious than thoseparallel to the tensile stress. Furthermore, a surface discontinuity whose plane isperpendicular to the tensile stress is more severe than if it were embedded (Barsom& Rolfe 1999). In partial penetration fillet-welded connections, a crack or gap is left due to thelack of penetration. Since this crack will be parallel to the direction of the bendingstress in beams, the gap will not open up under the application of stress. Similarly,consider an I-shaped beam with a cover plate fastened to the beam flanges bybolts. Now the region between bolt lines constitutes a ‘flaw’ or ‘crack’. But, sinceit is parallel to the stress field, it will not affect the strength of the member. Broadlyspeaking, any mechanical detail with bolts has a better fatigue life than does itsequivalent welded detail. Moreover, the inspection for defects in welding is moredifficult than in fastened detail. Similarly, the repair of a welded joint is moredifficult than a fastened joint.Stress ratio and frequency of cyclic loading From a large amount of testspecimens, it has been found that the stress ratio R has little influence on the fatiguebehaviour of welded components (Fricke 2003). This is so because tensile residualstresses up to yielding are expected at the critical crack initiation points of thewelded structures. Then the stress cycles remain tensile, irrespective of the R valuesof the external load. Therefore, the influence of the stress ratio is only taken intoaccount very cautiously or not at all in the codes or regulations (Lu & Mäkeläinen2003). The fatigue limit (see Section 17.4.3) for R = –1 is found to be about
- 9. Fatigue-resistant Design 17.9one-half of the tensile strength of steel (Gaylord et al. 1992). The effect of minimumstress (due to dead loads) is considered negligible for design purposes. Thefrequency of loading also does not influence the fatigue strength when the appliedstress range is low and the frequency is less than 50 Hz. However, when the stressrange is high, an increase in frequency may increase the fatigue strength.Influence of post-weld treatment Using the post-weld treatment of the weld, it ispossible to improve the fatigue strength of welded joints considerably, especiallythe fatigue limit. The improvement mainly involves an extension of the crackinitiation life and can be achieved by the following measures (Fricke 2003): l A reduction in the stress peak related to the weld shape l Removal of crack-like weld imperfections at the weld toe l Removal of detrimental tensile residual stresses, up to the formation of favourable compressive residual stresses in the area susceptible to crack initiation Post-weld treatment is of particular interest in connection with the repair offatigue cracks. However, it must be guaranteed that the fatigue strength of the areawhich is not subjected to post-weld treatment is high enough.17.2 Different Approaches to Fatigue AnalysisThe first known investigators concerned with fatigue phenomena were designersof axles for locomotives. Wöhler’s experiments with axles during 1852–60 werethe first known laboratory tests with the objective to derive and quantitativelydescribe the limits for fatigue. This was followed by more elaborate analyses ofstresses and their effects on fatigue by Berber, Goodman (during 1899), and others.Prof. August Thum and Prof. Ernst Gassner of the University of Darmstadt coinedthe word Betriebsfestigkeit (structural stability) in 1941 and formulated a procedurefor the experimental simulation of variable amplitude loading. Prof. Kurt Kloeppelin 1950s published allowable stresses for design details used in overhead cranesand railway bridges. The development of theories on the effects of plasticdeformation on fatigue resulted in the strain method discovered by Manson andCoffin in 1954. The theory of crack propagation was started by Griffith andcontinued by Paris and others in 1961. Fatigue was incorporated into design criteriatowards the end of the nineteenth century and has been extensively studied sincethen (Lu & Mäkeläinen 2003). According to the definition of the fatigue life, the approaches for fatigue analysiscan be classified into (1) the stress method, (2) the strain method, and (3) the crackpropagation method. Stress and strain methods characterize the total fatigue life in terms of cyclicstress range or strain range. In these methods, the number of stress or strain cyclesto induce fatigue failure in an initially uncracked or smooth surfaced laboratoryspecimen is estimated under controlled cyclic stress or strain. The resulting fatiguelife includes the fatigue crack initiation life to initiate a dominant crack and apropagation of this crack until catastrophic failure. Normally, the fatigue initiation
- 10. 17.10 Design of Steel Structureslife is about 90% of the total life due to the smooth surface of the specimen (Suresh1998). Under a high-cycle (> 102 to 104) low-stress fatigue situation, the materialdeforms primarily elastically and the failure time has traditionally been describedin terms of stress range. However, stresses associated with low-cycle fatigue(< 102 to 104) are generally high enough to cause plastic deformation prior tofailure. Under these circumstances, the fatigue life is described in terms of thestrain range. The low-cycle approach to fatigue design has found particularlywidespread use in ground vehicle industries (Socie & Marquis 2000). The basic premise of crack propagation method (fracture mechanics approach)is that all engineering components are inherently flawed. The size of a pre-existingflaw is generally determined from non-destructive flaw detection techniques, suchas visual, dye-penetrant, or x-ray techniques, or the ultrasonic, magnetic, or acousticemission methods. The fatigue life is then defined as the number of cycles topropagate the initial crack size to a critical size. The choice of the critical size ofcracks may be based on the fracture toughness of the material, the limit load forthe particular structural part, the allowable strain, or the permissible change in thecompliance of the component. The prediction of fatigue life is mainly based onlinear elastic fracture mechanics. The crack propagation method, which is aconservative approach to fatigue, has been widely used in fatigue-critical applicationswhere catastrophic failures will result in the loss of human lives, such as aerospaceand nuclear industries (Socie & Marquis 2000). The strain method and the crack propagation method are outside the scope ofthis book and we will confine our attention to the stress method, which is followedby the IS: 800. Interested readers may consult literature Lu and Mäkeläinen (2003),Gurney (1979), Fricke (2003), and Suresh (1998) for the details of other methods.Before discussing the stress method using S-N curves, let us discuss the parametersinvolved in constant-amplitude fatigue loading.17.3 Fatigue LoadingStructural components are subjected to two kinds of load history in fatigue design.The simplest load history, which occurs in machinery parts such as shafts and rodsduring periods of steady-state rotation is the constant-amplitude loading (seeFig. 17.9) and has the following parameters. Fig. 17.9 Terminology used in constant amplitude loading
- 11. Fatigue-resistant Design 17.111. Applied stress range f, which is the algebraic difference between the maximum stress fmax and the minimum stress fmin in the cycle, i.e., f = fmax – fmin (17.2)2. Mean stress, which is the algebraic mean of fmax and fmin in the cycle, i.e., fm = ( fmax + fmin)/2 (17.3)3. Stress amplitude, which is half the stress range in a cycle, i.e., fa = ( fmax – fmin)/2 (17.4)4. Stress ratio, which represents the relative magnitude of the minimum and the maximum stress in a cycle, i.e., R = fmin /fmax (17.5)The values of R corresponding to various loading cases are shown in Fig. 17.10.Thus R = 0 denotes stress ranging from zero to tension; R = –½ denotes stressalternating between tension and compression equal to half the tension, etc. Thestress fluctuation from a given minimum tensile load to a maximum tensile load ischaracterized by a positive value between 0 and 1 (0 < R < 1). Fig. 17.10 R-ratios for various loadings The second load history is the variable-amplitude loading history, in which theprobability of the same sequence and magnitude of stress ranges recurring duringa particular time interval is very small and cannot be represented by an analyticalfunction (see Fig. 17.11). This type of loading is experienced by many structures,such as wind loading on aircraft, wave loading on ships and offshore platforms,and truck loading on bridges. Stress Time Fig. 17.11 Variable-amplitude loading history
- 12. 17.12 Design of Steel Structures Either constant-amplitude loading or variable-amplitude loading can causeunidirectional stresses in structural components, such as pure tension andcompression, pure bending, or pure torsion. For the components with complicatedgeometries the resulting stresses may be in different directions. We are consideringonly unidirectional cases in this book. The effect of multi-axial loading may befound in the work by Socie and Marquis (2000).17.4 Stress MethodsIn the case of static loading, the yield strength or ultimate strength of the materialis obtained from tensile loading. The structural members are designed accordingto these values. Similarly, under the fluctuating loads, the significant strength isthe fatigue strength or fatigue limit. The fatigue strength is defined as the range ofcyclic stress a material can withstand for a given number of cycles without causingany failure (see Fig. 17.12). The fatigue limit or endurance limit is defined as themaximum value of the stress range that can be repeated an infinite number of timeson a test specimen without causing failure (see Fig. 17.12). It is generally consideredto correspond to a fatigue life of about 2 to 5 million cycles for ferrous alloys. Fig. 17.12 Typical S-N curves for ferrous and non-ferrous alloys In stress methods, it is necessary to determine the fatigue strength and/or fatiguelimit (analogous to yield strength) for the material so that cyclic stresses can bekept below that level to avoid fatigue failure for the required number of cycles.The structural components are designed in such a way that the maximum stressnever exceeds the materials fatigue strength or fatigue limit. Thus the stresses andstrains remain in the elastic region such that no local yielding occurs to initiate acrack.17.4.1 S-N CurvesThe most common way to describe the fatigue testing data is using S-N curves thatshow the relationship between the number of cycles, N, for fracture and themaximum stress, S, or stress range, ff, due to the applied cyclic load. Generally, the
- 13. Fatigue-resistant Design 17.13abscissa is the logarithm of N and the ordinate may be S, the stress or stress rangeff or the logarithm of stress or stress range. The stress to be calculated is simply the nominal stress at the location of thedetail (which can be determined from the applied loading such as forces andmoments and the cross-sectional properties of a component, based on the basictheory of the strength of materials). This simple representation of stress is possiblebecause we can include the effect of stress concentration in the selection of detailitself. Another approach is the notch stress method in which the local maximum stressdue to stress risers is calculated using the notch factor and nominal stress (Lu &Mäkeläinen 2003). This method requires the knowledge of the stress distributionin the vicinity of the weld, which is usually obtained by means of a finite elementanalysis. More discussions on the notch stress method could be found in the literatureby Fricke (2003) and von Wingerde et al. (1995). Since fabricated steel structures always contain a high magnitude of residualstresses, it is always preferable to use stress range, rather than the maximum stressor stress ratio, as the parameter to indicate the failure. A typical standard S-N curve is shown in Fig. 17.12. Most of the fatigue testsare performed in the high-cycle fatigue domain, where a linear relationship betweenthe stress range and the fatigue life exists in a log-log diagram. This linear relationshipcan be expressed as log N = log C – m log ff (17.6)where N is the number of cycles to failure, C is a constant, ff is the fatigue strengthdependent on detail category, and m is the slope of the fatigue strength curve witha value of 3 and/or 5.Alternatively, Eqn (17.6) can be written as N = NR( ff /fR)–m (17.7)where ff is the fatigue strength at loading cycle N (dependent on detail category),fR is the characteristic value of the fatigue strength at loading cycle NR (NR = 2 ¥106 or 5 ¥ 106), and m is the slope of the fatigue strength curve.Equation (17.7) can be rearranged as per the equation given in the code as ff = fR(NR/N)1/m (17.8) In order to obtain the meaningful engineering data, a large amount of testingshould be carried out. However, even though the same specimen is used in thefatigue tests, the results show a wide range of dispersion. This is due to the differentgeometrical micro-irregularities of surfaces for the same type of specimen. Thesedifferent local concentrations cause different fatigue lives. Therefore, it is necessaryto carry out the statistical analysis of fatigue data. This in turn makes it necessaryto consider the effect of failure probability. The curves formed by integrating thefailure probability into the S-N curve are called P-S-N curves (Lu & Mäkeläinen2003). The standard S-N curve provided in codes corresponds to a 50% probabilityof failure, i.e., P = 0.5 (Lu & Mäkeläinen 2003).
- 14. 17.14 Design of Steel Structures The main objective of the fatigue analysis is to design the structural componentsfor an infinite life or for a limited life. The objective of the infinite life design is toensure that the working stress due to loading is below the fatigue limit. Whereasthe objective of the limited life design is to predict the number of cycles availablewithin the fatigue life based on the stress level, or conversely to determine thestresses on a given number of cycles (Gaylord et al. 1992). It is seen from Fig. 17.12that the fatigue life reduces with increase in the stress range and at a limiting valueof stress, called fatigue limit or endurance limit, the curves flattens out. For normal steel and many ferrous alloys, the ‘knee’ point of the fatigue limit isnormally in the range of 105–107 cycles after which failure does not occur. Manyhigh-strength steels, aluminum alloys, and other materials do not generally exhibita knee point of the fatigue limit. For these materials, the fatigue limit is defined atthe stress level corresponding to 107 cycles (Suresh 1998). It has to be noted that the following factors affect the S-N curve: change inmechanical properties or microstructure of the material, chemical environment,cyclic frequency, temperature, residual stress, and surface effects (Lu & Mäkeläinen2003; Maddox 2005).17.4.2 Safe-life and Fail-safe Concepts of Structural Design‘Fail-safe’ and ‘safe life’ are the two concepts of fatigue-resistant structural design(Lu & Mäkeläinen 2003). In the safe-life method, the designer starts by making anestimation of the load spectrum to which the critical structural components arelikely to be subjected in service. These components are then analysed or testedunder that load spectrum to obtain their expected life. Finally a factor of safety isapplied in order to give a safe life during which the possibility of a failure due tofatigue is considered to be sufficiently remote. It is clear that by making the safetyfactor sufficiently large, the designer can govern the probability of the failureassociated with his/her design. On the other hand, if a fatigue crack does occur, itmay well be catastrophic, and safety depends on achieving a specified life withouta fatigue crack developing. In this method, the emphasis is on preventing the crackinitiation (Lu & Mäkeläinen 2003). In the fail-safe concept, the basis of design is that even if a crack in the mainmember does occur, there will always be sufficient strength and stiffness in theremaining members to enable the structure to be used safely. This concept impliesthat periodic in-service inspection is a necessity, and that the methods used mustbe such as to ensure that cracked members are discovered so that repairs orreplacements can be made. It is clear that with the fail-safe method of design the probability of partialfailure is much greater than with the safe-life design. In developing a fail-safestructure, the safe life should also be evaluated, in order to make sure that it is ofthe right order of magnitude. However, the emphasis, instead of being on theprevention of crack initiation, is on producing a structure in which a crack willpropagate slowly and which is capable of supporting the full design load afterpartial failure. The basic principle of the fail-safe design is therefore to produce amultiple load-path structure and preferably a structure containing crack arresters.In addition, the structural elements must be arranged so as to make inspections as
- 15. Fatigue-resistant Design 17.15easy as possible. In areas where this is not possible, the elements must be oversizedso that either fatigue cracking does not occur in them or the fatigue crack growth isso slow that there is no risk of failure (Lu & Mäkeläinen 2003).17.4.3 Using S-N Methods to Evaluate Fatigue LifeSeveral S-N methods are available for estimating the fatigue life of weldedcomponents: nominal stress method, structural hot spot stress method, notch stressmethod, notch stress intensity method, and notch strain method (Fricke 2003).Fatigue assessment according to the nominal stress method uses several S-N curvestogether with detail classes of basic joints. This is the simplest and most commonmethod adopted for estimating the fatigue life of structural joints and elements.The Eurocode 3-1993, Canadian code CAN/CSA-S.16.1, 2001, and the Indiancode IS: 800 are based on this method. The fatigue strength in IS: 800 is defined by a series of log ff – log N or logtf – log N curves (see Figs 17.13 and 17.14), each applying to a typical detailcategory. Each category is designated by a number which represents the referencevalue ffn (normal fatigue stress range) at 2 million cycles, i.e., the number of stresscycles, Nsc = 2 ¥ 106. The values are rounded values. Some common detail typesand their fatigue categories are provided in Table 13.3(1) to Table 13.3(4) of thecode. Figure 17.14 shows a few detail category classifications as per IS: 800. Twoother concepts are depicted in Fig. 17.13. One is the constant-amplitude fatiguelimit fd, which is the limiting stress range value above which a fatigue assessmentis necessary. The number of cycles corresponding to constant amplitude fatigue Fig. 17.13 S-N curves for normal stress as per IS: 800
- 16. 17.16 Design of Steel Structures Constructional details Detail category Illustration (see note) Description Welded plate I-section and box girders with continuous longitu- dinal welds (8) & (9) zones of continuous auto- 92 matic longitudinal fillet or butt welds carried out from both sides and all welds not having un-repaired stop– start positions. Welded plate I-section and box girders with continuous longitu- dinal welds (10) & (11) zones of continuous automatic butt welds made from one side only with a continuous backing bar and all welds not having un- 83 repaired stop–start positions. (12) Zones of continuous longitu- dinal fillet or butt welds carried out from both sides but containing stop– star t positions. For continuous manual longitudinal fillet or butt welds carried out from both sides, use Detail Category 92. Welded plate I-section and box girders with continuous longitu- dinal welds 66 (13) Zones of continuous longitu- dinal welds carried out from one side only, with or without stop–star t positions. Fig. 17.14 Detail category classifications as per IS 800 : 2007limit is 5 million cycles, i.e., Nd = 5 ¥ 106. The other is cut-off limit, fL, which is alimit below which stress ranges of the design spectrum do not contribute to thecalculated cumulative damage. The number of cycles corresponding to this valueis 108 cycles, i.e., NL = 108. The cut-off limit is specified because when variable-amplitude loading is applied, the stresses less than the fatigue limit still causedamage due to the fact that larger amplitude cycles may start to propagate thecrack. The fatigue strength curves for nominal stresses are defined by Eqn (17.6) orEqn (17.8). The constant representing the slope of the fatigue strength curves, m,is taken as 3 and/or 5, and log C is a constant that depends on the related part of theslope. Their values are given in Table 17.1. Similar fatigue strength curves areused for shear stresses (Fig. 17.15) and only one slope value is taken, i.e., m = 5.
- 17. Fatigue-resistant Design 17.17Table 17.1 Numerical values for fatigue strength curves log C for N < 108 Stress range at constant- Stress range at cut- amplitude fatigue limit off limitNormal stress rangeffn (N/mm2) N £ 5 ¥ 106 N > 5 ¥ 106 fd (N/mm2) fL (N/mm2) (m = 3) (m = 5) 160 12.901 17.036 118 64 140 12.751 16.786 103 57 125 12.601 16.536 92 51 112 12.451 16.286 83 45 100 12.301 16.036 74 40 90 12.151 15.786 66 36 80 12.001 15.536 59 32 71 11.851 15.286 52 29 63 11.701 15.036 46 26 56 11.551 14.786 41 23 50 11.401 14.536 37 20 45 11.251 14.286 33 18 40 11.101 14.036 29 16 36 10.951 13.786 27 14Shear stress rangetfn (N/mm2) N < 108 (m = 5) td (N/mm2) tL (N/mm2) 100 16.301 83 46 80 15.801 67 36Source: (Lu & Mäkeläinen 2003; Eurocode 3, 1992) Fig. 17.15 SN curves for shear stress as per IS 800 : 2007
- 18. 17.18 Design of Steel StructuresThese curves are based on representative experimental investigations and thusinclude the effects of local stress concentrations due to the weld geometry, sizeand shape of acceptable discontinuities, the stress direction, residual stresses,metallurgical conditions, and, in some cases, the welding process and the post-weld improvement procedures (Lu & Mäkeläinen 2003).No fatigue assessment is required when any of the following conditions is satisfiedaccording to the code: 1. The largest nominal stress range ff max satisfies ff max £ 27mc /gmft (17.9) where mc is a correction factor [see Eqn (17.12)] and gmft is the partial safety factor for fatigue strength (see Table 17.2) 2. The highest shear stress range tmax satisfies tf max £ 67mc /gmft (17.10) 3. The total number of actual stress cycles, Nsc, satisfies Nsc £ 5 ¥ 106 [27mc /(gmft ffeq)]3 (17.11)In these conditions, ff eq is the equivalent constant-amplitude stress range (MPa),which is defined as the constant-amplitude stress range that would result in thesame fatigue life as for the spectrum of variable-amplitude stress ranges, when thecomparison is based on Miner’s summation (see Section 17.5). gmft is the partialsafety factor for fatigue loading and its value has to be taken as per Table 17.2.Table 17.2 Partial safety factors for fatigue strength (gmft) Inspection and access Consequence of failure Fail-safe Non-fail-safePeriodic inspection and maintenance, accessibilityto detail is good 1.00 1.25Periodic inspection and maintenance, poor accessi-bility for detail 1.15 1.35 The code also recommends a partial safety factor for loads on the evaluation ofthe stress range in fatigue design as 1.0. The design stress should be determined bythe elastic analysis of the structures by using conventional stress analysis methods.The normal and shear stresses should be determined considering all design actionson the members, but excluding the stress concentration due to the geometry of thedetail. The code stipulates that the stress concentration not characteristic of thedetail should however be accommodated in the stress calculation. In the fatigue design of trusses made of members with open cross sections andnot having pinned ends, the stresses due to secondary bending moments should betaken into account unless the slenderness ratio (KL/r) of the member is less than40. To take into account the influence of the thickness of the plate, the code gives acapacity reduction factor mc which should be applied when plates of thicknessesmore than 25 mm are joined together by transverse fillet welds: mc = (25/tp)0.25 £ 1.0 (17.12)
- 19. Fatigue-resistant Design 17.19where tp is the actual thickness (in mm) of the thicker plate being jointed. Thisreduction should be applied only to structural details with welds transverse to thedirection of normal stresses (Eurocode 3 1992). Also when the detail category inthe classification tables of the code already varies with thickness, the abovecorrection for thickness should not be applied (Eurocode 3 1992). The fatigue strength of the standard detail of the normal fatigue range notcorrected for the effects discussed above is given by the code as below:When Nsc ≤ 5 ¥ 106, ff = ffn 3 5 ´ 106 /N sc (17.13)when 5 ¥ 106 £ Nsc £ 108, ff = ffn 5 5 ´ 106 /N sc (17.14)Similarly, the shear fatigue stress range is given by the code as tf = tfn 5 5 ´ 106 /N sc (17.15)where ff and tf are the design normal and shear fatigue stress ranges of the detail,respectively, for life cycle of Nsc and ffn and tfn are the normal and shear fatiguestrengths of the detail for 5 ¥ 106 cycles. At any point in the structure, if the actualnormal and shear stress ranges, f and t, are less than the design fatigue strengthrange corresponding to 5 ¥ 106 cycles, with an appropriate safety factor, no furtherassessment for fatigue is necessary at that point. It has to be noted that the absolute maximum value of the normal and shearstresses should never exceed the elastic limit ( fy, ty) for the material under staticloading. The maximum stress range shall not also exceed 1.5fy for normal stressesand 1.5fy / 3 for shear stresses under any circumstances as per the code. The codealso states that the actual normal and shear stress range, f and t, at a point of thestructure subjected to Nsc cycles in life shall satisfy f £ ffd = mc ff /gmft (17.16)and t £ tfd = mctf /gmftwhere mc is the correction factor defined by Eqn (17.12), gmft is the partial safetyfactor against fatigue failure as given in Table 17.2, and ff and tf are the normaland shear fatigue ranges for the actual life cycle Nsc as given by Eqns (17.13)–(17.15).17.4.4 Modified Goodman DiagramAs we have seen in Figs 17.13 and 17.15, the S-N curves are generated with fullyreverse load (R = –1) and zero mean stresses. However non-zero mean stresses can
- 20. 17.20 Design of Steel Structuresalso play an important role in resulting fatigue data. Also for the purpose of designit is more convenient to have the maximum and minimum stresses for a given lifeas the main parameters. The modified Goodman diagram, as shown in Fig. 17.16,provides this kind of information. This is a variation of the diagram published byGoodman in 1899. In this diagram, the maximum stresses are plotted in the verticalordinate and minimum stresses as abscissa. Each curve in the diagram is the locusof all the points corresponding to a given fatigue life, and the diagram covers thefull range of stress ratios –1 £ R £ 1. Radial lines from the origin correspond to thevarious stress ratios. Since R = 1 denotes no reversal of stress, the radial line R = 1corresponds to static tension and all the curves for a given steel join at the intersectionof R = 1 with the ordinate correspond to the tensile stress of the steel. It is also seenthat the fatigue life decreases with increasing stress magnitude or stress range.Fig. 17.16 Modified Goodman diagram showing variation of fatigue life with stress magnitude and range (Trahair et al. 2001) Taking yield stress as the limiting useful strength, the curves in Fig. 17.16 canbe represented closely by the straight lines AB and BC of Fig. 17.17. This enablesfatigue–design criteria to be put in the form of simple equations. Allowable stressFig. 17.17 Goodman diagram with straight line representation (Gaylord et al. 1992)
- 21. Fatigue-resistant Design 17.21formulas may be obtained by a factor of safety to ABC to get DEF. This factor ofsafety can be smaller than the factor of safety for static load because of the smallerprobability of the occurrence of the much larger number of cycles of the service-load magnitude needed to cause a fatigue failure (Gaylord et al. 1992).17.5 Fatigue Assessment for Variable Stress RangesUntil now, we discussed about fatigue properties of structural elements under aconstant amplitude. But in real situations, stress ranges of different magnitudestake place at the detail and these stress ranges are applied for various lengths oftime. For example, if a crane is carried by a continuous beam over severalintermediate supports, more than one stress cycle will be applied per trip at a givenlocation. This is because loading adjacent spans causes stress cycles in addition tothe cycle created when the crane passes directly over the location underconsideration. For this general case, one trip is termed loading event and the stressvariation at a given point in the structure during such an event is called stresshistory (Kulak & Gilmor 1998). A state-of-the-art review on the fatigue crackgrowth analysis under variable-amplitude loading is available in Murthy et al.(2004). Though both linear and non-linear damage theories are available, the lineartheory first proposed by Palmgren in 1924 and further developed by Miner in 1945is used in structural engineering applications (Bannantine et al. 1990). This methodis easy to understand and apply and found to give satisfactory results.17.5.1 PalmgrenMiner RuleThe fatigue life of a component under variable-amplitude loading can be calculatedusing the Palmgren–Miner rule, which is a linear damage rule and assumes that 1. the damage fraction that results from any particular stress range level is a linear function of the number of cycles that takes place at the stress range, and 2. the total damages from all stress range levels that are applied to the detail is the sum of all such occurrences.If ni is the required number of cycles corresponding to the stress amplitude fi in asequence of m blocks and Ni is the number of cycles to failure at fi , then thePalmgren–Miner rule states that the failure would occur when m å ni /Ni £ k (17.17) i =1and Di = 1/Ni (17.18)where Di is called the damage of a single cycle at stress level fi . The scheme ofPlamgren–Miner’s rule is shown in Fig. 17.18. The rule was first introduced byPalmgren in the analysis of ball bearings and was adapted by Miner for aircraftstructure (Lu & Mäkeläinen 2003). The value of k is experimentally found to varybetween 0.7 and 2.2. Usually for design purposes, k is assumed to be equal to 1.
- 22. 17.22 Design of Steel Structures Fig. 17.18 Scheme of PalmgrenMiners rule The code gives the following rule based on the Palmgren–Miner rule. The fatigueassessment at any point in a structure, where in variable stress ranges ff i or tf i for ninumber of cycles (i = 1 to r ) are encountered, shall satisfy the following:(a) For normal stress ( f ) g5 r å ni fi3 å n j f j5 i =1 j = g5 + £ 1.0 (17.19) 5 ´ 10 ( m ffn /g mft ) 6 3 5 ´ 10 ( m ffn /g mft )5 6(b) For shear stresses (t) r å nit 5 £ 5 ´ 106 (mt fn /g mft )5 fi (17.20) i =1where g5 is the summation upper limit of all the normal stress ranges ( fi ) havingmagnitudes lesser than (mc ffn /gmft) for that detail and the lower limit of all thenormal stress ranges ( fj ) having magnitudes greater than (mc ffn /gmft) for the detail.In the above summation all normal stress ranges ( fi and ti) having magnitudes lessthan 0.55mc ffn, and 0.55mctfn may be disregarded. It should be noted that, when variable-amplitude loading is applied, the stresseslesser than the fatigue limit still cause damage due to the fact that larger amplitudecycles may start to propagate the crack. However, the linear Palmgren–Miner ruleassumes independence of damage accumulation. Empirically, tests have shown that differences exist between low–high sequencesand high–low sequence. Thus, there are two main shortcomings of the linear damagerule: assuming sequence independence and damage accumulation independence.These two shortcomings might be overcome by non-linear damage rules. Also, instructural engineering applications where residual stresses are high and plasticityis restricted, the two factors were found to have small influence (Kulak & Gilmor1998). Hence the Palmgren–Miner rule is suggested by several codes to accountfor cumulative damage. It is often convenient to express the Palmgren–Miner rulein terms of an equivalent stress range as follows (Kulak & Gilmor 1998): ff eq = S(ni ffm/Sni)1/m (17.21)
- 23. Fatigue-resistant Design 17.23The code gives the following expression for the same: 1/3 é g5 r ù ê å ni f fi + å n j f fj 3 5 ú ff eq = ê ú i =1 j =g5 (17.22) ê ë n ú û gwhere n = å ni (17.23) i =117.5.2 Cycle CountingWhen using the linear Palmgren–Miner rule to estimate the fatigue life, the variable-amplitude loading has to be transformed into a series of constant-amplitude loadings.Several methods are available to do cycle counting: reservoir counting, level crossingcounting, peak counting, simple range counting, and rainflow counting. In thissection, we only provide the details of rainflow counting (this algorithm was firstdevised by Tatsuo Endo and M. Matsuiski in the year 1968 and is more popularthan the other methods of cycle counting). Rainflow is a generic term to describeany cycle counting method that identifies closed hysteresis loops in the stress–strain response of material subjected to cyclic loading. Several algorithms areavailable to perform the counting; however, they all require that the entire loadhistory be known before the counting process starts (Downing & Socie 1982). Themethodology followed in rainflow counting follows. 1. In order to eliminate the counting of half cycles, the load history has to be drawn starting and ending at the greatest magnitude. 2. The flow of rain has to be stopped when (a) The rain begins at a local maximum and falls opposite a local maximum that is greater than the starting point. (b) The rain encounters a previous flow.Figure 17.19 illustrates the procedure of cycle counting using rainflow method.The counting is first started from the tension peaks. The details of counting basedon this rule are described next. l Route 1 starts from A and falls down at B. Since the value of C is less than that of A, the rain can continue and fall down to line CD. Similarly, since the value of A is larger than that of E, C, I, K, and M, it will stop at the position shown in Fig. 17.19(b). This procedure is carried out based on rule (a). l Route 2 starts from C and stops as shown in Fig. 17.19(b) due to its encounter with the previous rainflow (Route 1). This illustrates rule (b). l Route 3 starts from E and stops due to the value of G being larger than that of E [rule (a)]. l Route 4 is based on rule (b). l Route 5 is based on rule (a). l Route 6 is based on rule (b). l Route 7 is based on rule (a).
- 24. 17.24 Design of Steel Structures Fig. 17.19 Scheme of rainflow counting (Lu & Mäkeläinen 2003) Similar rainflow counting from compression peaks is shown in Fig. 17.19(c).Figure 17.19(d) shows the cycles from both the tension side and the compressionside. This can be done as follows. Start from Route 1 of the tension side and find the ending point of Route 1.Then check the ratio of the compression side that starts from this point. In this caseit is Route 6¢. This is one cycle of loading. Similarly, other cycles in the loadinghistory are obtained as shown in Fig. 17.19(d). After this counting, the stress range and the number of cycles corresponding tothe stress range are obtained and the damage can be estimated according toPalmgren–Miner’s rule. Rainflow counting is easy to do manually for simple loadinghistories; however, for complex loading histories, numerical methods are to beused (Downing & Socie 1982). The details of other counting methods may befound in Gurney (1979) and Maddox (2005). In the reservoir method, it is assumed that the troughs in the variable-amplitudeloading history (see Fig. 17.11) act as reservoirs and for each ‘peak’ the lowest‘trough’ drains the water. A tabular format is set up to count these reservoirs.Deducting the trough value of the stress from the peak value of the stress, thestress range in each reservoir is found. The damage resulting from each of thesestress ranges is calculated using Eqns (17.6) and (17.17) and Fig. 17.13. Thecumulative value of ni /Ni suggests whether the detail is safe or not. Example 17.4(at the end of this chapter) explains the use of the reservoir method.17.5.3 Fatigue Assessment of Hollow SectionsThe member force for hollow sections according to the code may be analysed
- 25. Fatigue-resistant Design 17.25neglecting the effect of eccentricities and joint stiffness and assuming hingedconnections, provided that the effects of secondary bending moments on the stressrange are considered. In the absence of a rigorous stress analysis and modelling ofthe joint, the effects of the secondary bending moment may be taken into accountby multiplying the stress range due to the axial member forces by appropriatecoefficients as given in Table 17.3 (for joints in lattice girders made from circularhollow sections) and Table 17.4 (for joints in lattice girders made from rectangularhollow sections). The values in these two tables are approximate empirical valuesor values based on testing.Table 17.3 Multiplying factors for calculated stress range as per IS: 800 for lattice girders made from circular hollow sections) Type of connection Chords Verticals DiagonalsGap K type 1.5 1.0 1.3Connections N type 1.5 1.8 1.4Overlap K type 1.5 1.0 1.2Connections N type 1.5 1.65 1.25Table 17.4 Multiplying factors for calculated stress range as per IS: 800 for lattice girders made from rectangular hollow sections Type of joint Chords Verticals DiagonalsGap K type 1.5 1.0 1.5Connections N type 1.5 2.2 1.6Overlap K type 1.5 1.0 1.3Connections N type 1.5 2.0 1.417.6 General Guidelines for Fatigue-resistant DesignFrom experience, it is seen that most of the fatigue failures are caused by improperdetailing rather than inadequate design. Indeed, weld deflects and poor weld detailsare the major contributors to fatigue failures (Radaj 1990). Hence the followingprecautions should be taken when designing and detailing structures (especiallywith welded joints) subjected to fatigue loads (McGuire 1968; Gurney 1979; Lu &Mäkeläinen, 2003; Maddox 2005). 1. Multiple load paths and/or structural redundancy should be provided in structures to avoid overall collapse of the structure due to the failure of one element under fatigue. 2. Abrupt change in the cross section or stiffness of members should be avoided. 3. Eccentricities should be avoided or they should be reduced to the minimum (Blodgett 1966). 4. Wherever practicable, joints and welds should be restricted to locations of low stress such as at points of contraflexure or near the neutral axis. 5. Details that produce severe stress concentrations or poor stress distribution should be avoided. For example, the fatigue strength of a complete penetration grove welded butt splice in a tension member increases if the weld is ground
- 26. 17.26 Design of Steel Structures flush with the surface of the connecting parts. This eliminates the stress concentration that arises in the as-welded condition. Grinding, however, should not be specified unless essential, since it adds to the final cost (Blodgett 1966). Figure 17.20(a) illustrates a transverse joint in which the weld is elongated in the direction of the load to produce a more uniform transfer of stress than in a conventional weld of Fig. 17.20(b). However, it has to be noted that the code does not permit an increase in the allowable unit stress of such a weld. Fig. 17.20 Stress concentration at the toe of a fillet weld 6. Re-entrant, notch-like corners should be avoided; wherever possible gradual change in sections should be provided to produce a smooth ‘stress flow’. 7. Detail that may introduce high, localized constraints should be avoided. 8. Instead of intermittent welds, continuous welds should be used. Intersection of welds should be avoided. 9. Wherever possible, butt or single- and double-bevel butt welds should be used instead of fillet welds. When fillet welds are selected, double-sided fillet welds should be preferred over single-sided fillet welds. Similarly, deep penetration fillet welds should be preferred over normal fillet welds.10. The size of fillet welds (carrying longitudinal shear) adopted at the site should not be larger than the designed size.11. Warping and residual stress build-up in butt welds should be minimized by proper edge preparation.12. Welded joints may be preheated or post-heated to relieve the residual stresses. However stress relieving the weld has been found to have no appreciable effect upon fatigue strength (Bennantine et al 1990).13. Attachments on parts subjected to severe fatigue loading should be avoided (Blodgett 1966). If unavoidable, they should be welded with a profile that merges smoothly with the profile of the parent metal.14. Suitable inspection should be provided during the fabrication and erection of structures, especially during welding and tightening of high-strength friction grip bolts.15. When fatigue cracks are discovered, steps to prevent their propagation should be taken immediately. The repair measures undertaken should not result in a more severe fatigue condition (Kulak & Gilmor 1998).16. At locations where heavy fatigue loading is expected, such as machine bases subject to dynamic loading or the end connections of large flare booms subjected to wind oscillations, HSFG waisted bolts should be employed. These bolts resist direct tension by means of the pre-stress in the bolts.
- 27. Fatigue-resistant Design 17.2717. Corrosion fatigue (especially in offshore structures) may be minimized by particular care in the choice of the material, design, fabrication technique, and the use of cathodic protection. Due attention must be paid to the correct range of potential for cathodic protection. Too low a potential leaves the material susceptible to corrosion fatigue. A too high potential allows hydrogen to enter, leading to the risk of hydrogen embrittlement, if the yield stress is sufficiently high (Clarke & Coverman 1987).17.6.1 Fatigue Cracking from Outofplane EffectsIn many instances, it was found that fatigue crack growth resulted from theimposition of relatively small, out-of-plane deformations (Fisher 1978; Kulak &Gilmor 1998). Such deformations can be eliminated by proper detailing. Forexample, normally transverse stiffeners in plate girders are welded to the web ofthe plate girders, leaving a small gap at the bottom as shown in Fig. 17.21. It isdone mainly to avoid the effect of stress concentration which will increase thefatigue or brittle fracture possibilities. It is also permitted in structural codes. Whenlateral movement of the top flange relative to the bottom flange takes place, largestrains are produced in the gap region due to the significant change in the stiffnessbetween the stiffened and unstiffened (gap) regions of the web. Due to these largestrains, only few cycles are required to propagate a crack (Fisher 1978; Fisher &Mertz 1985). Figure 17.21 shows such a crack emanating from the weld toe at thebottom of the stiffener. This crack may also extend across the toe of the fillet weldat the underside of the stiffener and for some distance into the web (Kulak &Gilmor 1998). However, it will not cause any problem, since it is parallel to thedirection of the main stress field of the girder in service. However, if the crack isnot arrested, it may grow and turn upwards or downwards in the web—which maybe an unfavourable orientation with respect to service-load stresses.Fig. 17.21 Fatigue cracking due to out-of-plane moment (Kulak & Grondin 2002)
- 28. 17.28 Design of Steel Structures Such flange movements and cracking are possible due to transverse forces inskew bridges. Similar out-of-plane movements have also been found in bridges asa consequence of shipping and handling of such girders. The detail shown inFig. 17.21 has been identified as a source of many fatigue crack locations in thepast (Fisher 1978; Keating 1994). One way of dealing with the crack is to drill ahole of 12 mm diameter in the web of the girder at the end of the crack as shown inFig. 17.22. It is important to locate and drill the hole at the extremity of the cracktip, such that the hole intercepts the crack front. If necessary, the hole should beground lightly to remove scratches and burrs. The hole should be left open andmonitored for any further crack growth. Sometimes, a high-strength bolt is placedin the hole and pre-tensioned—which will introduce high compressive stresses inthe web, thus effectively increasing the fatigue life of this region (Kulak & Gilmor1998). However, if the original fatigue crack continues to grow, it will be knownonly after it appears beyond the bolt head or washer. Hence it is better to leave thedrilled hole open for easy monitoring. Fig. 17.22 Repair of a fatigue crack (Kulak & Grondin 2002) Similar out-of-plane movements may occur in a floor beam attached to aconnection plate that is welded to the web of the girder as shown in Fig. 17.23. Insuch a situation, the floor beam tends to rotate under the traffic load. This results ina deformation within the gap at the top of the connection plate (Fisher 1978; Fisher& Mertz 1985). This out-of-plane movement will result in fatigue cracks at theweld at the top of the connection plate or at the web-to-flange fillet weld of the Fig. 17.23 Floor beam-to-girder connection (Kulak & Grondin 2002)
- 29. Fatigue-resistant Design 17.29girder, or both, under relatively few cycles of load. Calculations show that a verysmall displacement, of the order of 0.003 mm, could significantly reduce the fatiguelife of this detail (Kulak & Gilmor 1998). Other sources of out-of-plane fatigue cracking include the following.Restraint at simple end conditions As discussed in Chapter 2, many simpleconnections designed based on the assumption that they will not transmit anymoment, in reality, carry some moment. Hence the connecting elements may deformunder the moment. Thus, end rotation at web framing angles causes the angles todeform and results in additional loads in the connecting bolts and/or rivets, whichare not considered in the design. Due to cyclic loading, fatigue cracks may developin the angles and also in the connecting bolts or rivets.Coped beams To facilitate easy connection, the ends of beams are often cut back(called coped) as shown in Fig. 17.24. In beams such ‘coped’ ends (flame cuttingthe top or bottom flange or both flanges), due to the small radius and unevennessof cutting, are susceptible to fatigue cracking. Normally, coped ends of the beamsare locations of zero moments. However, due to the restraint offered by theconnection, fatigue cracking may result. Hence, as far as possible, coped endsshould be avoided. More information on the design of beams with coped ends maybe found in Cheng (1993).Fig. 17.24 Bottom flange of floor beam coped at connection to girder (Kulak & Grondin 2002)Bracing connections Lateral bracing attached to horizontal connection plates weldedto girder webs also produces out-of-plane flexing of the web and results in fatiguecracking of the connection welds.17.7 Fatigue Assessment Under Combined StressesWhen both normal and shear stresses are concurrently present in considerablemagnitudes at a given location during a given loading event, the principal stressesshould be calculated and the stress range corresponding to those stresses should beused in the fatigue life evaluation. (Normal stress may be defined as the stressperpendicular to the direction of the potential fatigue crack.)
- 30. 17.30 Design of Steel Structures When normal and shear stresses are present at the same location but do notoccur simultaneously under a given loading event, Kulak and Gilmor (1998) suggestthat the individual components of damage can be added using Miner’s summationas below: [ fe /ffd]3 + [te /tfd]5 £ 1 (17.24)where f and t refer to normal stresses and shear stresses, respectively. The subscript‘e’ denotes a calculated equivalent stress range [see Eqns (17.21)–(17.23)] and thesubscript ‘fd’ refers to the design fatigue strength for the detail.17.8 Fatigue Analysis of Building FramesA fatigue analysis is not presently required for steel structures subjected to wind orearthquakes. Seismic design, as currently prescribed in IS: 800 and other codes,refers mainly to the provision of stiffness, strength, and ductility. The latter isrequired due to the fact that structural elements are allowed to yield during strongearthquakes. However, such a design methodology inevitably accepts structuraldamage due to the development of inelastic action. In spite of the recognition ofthis fact, the fatigue limit state is not introduced in the codes. One reason, of arather practical nature, is that from the past experience steel structures were notconsidered vulnerable to earthquake. Another reason is that despite the similaritiesto the usual fatigue mechanisms, i.e., formation and growth of fatigue cracks, thereexist differences to the fatigue due to the usual dynamic loading. That is, fatiguedue to earthquake loading is not due to a large number of applied cycles of ratherlow nominal stress, but due to a small number of applied inelastic deformationcycles, i.e., it is a case of low-cycle fatigue. This difference calls for a differentassessment procedure of the phenomenon (unlike for high-cycle fatigue), on whicha generally accepted agreement is yet to be found. However, after the Northridge, USA (1994) and Kobe, Japan (1995) earthquakes,it was found that in many cases brittle fractures are initiated within the connectionsat low levels of plastic demands (and in some cases, especially Northridge) whilethe structure remained elastic. Extensive analytical and experimental investigationsundertaken after these earthquakes revealed that the poor fatigue resistance due tothe low material toughness, poor weld execution, high stress concentration of details,restraint conditions, high strain rates, low temperature, etc., were the main causesof failure. Failures were found in regions where high inelastic action develops,such as in the region of beam-to-column-joints. They include rigid weldedconnections, rigid and semi-rigid bolted end-plate connections, top and seat angleconnections, and compact or slender web panels. Structural members outside jointregions have also been found to be prone to fatigue failure when subjected tocycles of inelastic deformations. Hence a fatigue assessment procedure similar to high-cycle fatigue curves ofFigs 17.13 and 17.15, but substituting deformation ranges instead of the stressranges, has been proposed by Vayas et al. (2003). The relevant fatigue expressionin this case is written as log N = log C – m log Dp (17.25)
- 31. Fatigue-resistant Design 17.31where Dp is the fatigue deformability (plastic rotation), N is the number of rotationrange cycles, m is the slope constant of a fatigue curve, and log C is a constant. A transformation of elastic and inelastic deformation into equivalent stresseshas also been proposed by Ballio and Castiglioni (1995). However, the fact thatthe resulting stresses may be well above the material tensile strength might beconfusing for the application. In the absence of more specific information, the damage assessment for variableranges of plastic rotation may be performed as for high-cycle fatigue in accordancewith the linear Palmgren–Miner cumulative law [Eqn (17.17)]. The value of m inEqn (17.25) ranges between 1.3 and 3.4 for welded connections and top and seatangle connections. For ‘log C’ values and other details of low-cycle fatigueassessment, the reader may consult Vayas et al. (2003), Ballio and Castiglioni(1995), Mazzolani (2000), Righiniotis et al. (2000) and Vayas et al. (1999). Table 17.5 summarizes the various possible formulations of the fatigue analysisas well as examples of relevant applications. Mohammadi (2004) gives details ofnon-destructive testing methods applied to the fatigue reliability assessment ofstructures.Table 17.5 Formulations of the fatigue rules Structural response Elastic Æ inelastic 4 8No. of cycles to failure ~10 –10 ~102–104 ~100–102Fatigue curves for ranges of Generalized Generalized total Generalized inelastic forces deformations deformationsUsual field applications Bridges, crane Slender plate Buildings under girders chimneys, girders seismic loading masts, etc.Source: Vayas et al. (2003)ExamplesExample 17.1 An overhead crane in a factory has a gantry girder with a simplysupported span of 6.0 m. The section used for the girder is ISMB 400. The capacityof the crane is 150 kN and the gantry girder receives a maximum of 80% of thetotal load as the reactive force. It is assumed that this force is applied to the girderas a single concentrated load. The crane operates 200 days/year and 8 hr/day.The crane makes a maximum of three trips per hour at this load level. The designlife of the building is 50 years. Is the fatigue life of this gantry girder satisfactory?SolutionNumber of stress cycles (equals number of load cycles in this case) N = (3 cycles/hr)(8 hr/day)(200 days/year)(50 years) = 240,000 cyclesDetail category and fatigue strengthThe provided beam corresponds to detail category 118 as per Table 13.3(1) of thecode. From Fig. 17.13, read the category 118 line at N = 240,000 cycles to find that
- 32. 17.32 Design of Steel Structuresuncorrected fatigue strength is 330 MPa. The fatigue strength of this detail canalso be calculated using Eqn (17.13) as ff = 118 ¥ 3 (5 ´ 106 / 240, 000) = 324.6 MPaAssuming fail–safe and poor accessibility for detail, gmft = 1.15Design fatigue strength = 324.6/1.15 = 282.26 MPaCalculation of actual stress range fmin = 0 M = PL/4 = (150 ¥ 103 ¥ 0.8) (6000)/4 = 180 ¥ 106 N mm fmax = M/Z = 180 ¥ 106/(1022.9 ¥ 103) = 176 MPa < fy = 250 MPaThus f = 176 – 0 = 176 MPa.Since the actual stress range (176 MPa) is less than the design fatigue strength(282.26 MPa) for this detail, the size of girder is safe. Shear force as support = 150 ¥ 103 ¥ 0.8/2 = 60,000 N Shear stress = SF/(dtw) = 60,000/(400 ¥ 8.9) = 16.85 MPa < (27/1.15 = 23.48 MPa)Hence fatigue assessment is not required at the support. However, let us find outthe fatigue strength in shear of the detail using Eqn (17.15). tf = tfn 5 5 ´ 106 /N sc = 118 5 5 ´ 106 / 240,000 = 216.58 MPaDesign fatigue strength in shear = 216.58/1.15 = 188.3 ? 16.85 MPaHowever, the following points have to be borne in mind. 1. The number of stress cycles will not always be equal to the number of load cycles. For example, in a continuous beam or when a multiple-axle vehicle transverses a member, more than one stress cycle could occur. 2. Since the stress due to the dead load is always present, the change in stress in the member could be taken equal to the change in stress produced by the moving (live) load. 3. Of course, we can also compare the number of cycles permitted at the actual stress range of 176 MPa.From Table 17.1, log C for category 118 and N < 5 ¥ 105 = 12.901From Eqn (17.6), log N = 12.901 – 3 log 176Thus N = 1,460,366 cyclesSince the actual number of cycles is only 240,000, this also shows that the size ofthe girder is sufficient.Example 17.2 After erecting the gantry girder of Example 17.1, it has been decidedfor the crane to accommodate two trips per hour at a load level of 180 kN, inaddition to the existing conditions. Will the fatigue life of this gantry girder be stillsatisfactory?
- 33. Fatigue-resistant Design 17.33SolutionNumber of cycles at the old load level, n1 = 240,000Number of cycles to failure at the old load level, N1 = 1460,366Number of cycles at the new load level, N2 = (2 cycle/hr)(8 hr/day)(200 days/year)(50 years) = 160,000 cycles < 5 ¥ 106 cyclesNumber of cycles to failure at the new load level M = PL/4 = (180 ¥ 103 ¥ 0.8)(6000/4) = 216 ¥ 106 N mm fmax = 216 ¥ 106/(1022.9 ¥ 103) = 211.2 MPa < fy = 250 MPaUsing Fig. 17.13 for category 118 or using Eqn (17.6), Log N2 = 12.901 – 3 log 211.2, N2 = 845, 119 cyclesChecking Eqn (17.18), Sni /Ni £ 1we get 240,000/1460,366 + 160,000/845,119 = 0.35Since the total effect of the two different stress ranges is less than 1.0, the gantrygirder is safe for the additional loading condition.Example 17.3 Use the equivalent stress method to determine the percentage of lifethat has been expended by the loading applied to the gantry girder of Example17.2. Note that the Palmgren–Miner cumulative fatigue damage rule [Eqn (17.17)]can be expressed in terms of an equivalent stress range fe (as per Kulak & Gilmor,1998) as fe = [Sai fem]1/m (17.26)where ai = ni /SNi (17.27)SolutionAll the necessary data as available from Example 17.2 are given below: n1 = 240,000, n2 = 160,000 f1 = 176 MPa, f2 = 211.2 MPa N = 240,000 + 160,000 = 400,000 cyclesUsing Eqn (17.26) fe = [(240,000/400,000)(176)3 + (160,000/400,000)(211.2)3]1/3 = 191.7 MPaThus the number of cycles to failure Log N = 12.901 – 3 log 191.7 or N = 1130,143 cyclesSince the actual number of cycles is 400,000, the percentage of life expended is(400,000/1130,143) ¥ 100 = 35%Note that we get the same result using Miner’s summation.Example 17.4 The numerical values of the peaks and valleys for the stress historyare shown in Fig. 17.25.
- 34. 17.34 Design of Steel Structures Fig. 17.25 Reservoir analysis of stress histories (Kulak & Grondin 2002) Peak/Trough no. Stress (in MPa) 1 96 2 15 3 47 4 10 5 80 6 10 7 35 8 15Apply the reservoir counting method in order to identify the stress ranges in thisstress spectrum and evaluate the effects of 3.0 million loading events of this stresshistory acting on a welded I-beam that uses longitudinal fillet welds to connect theflanges to the web.SolutionThis detail is category 92 as per Table 26b of the code (see also Fig. 17.14). Thereservoir counting method is presented in a tabular form. Drain from trough no. Water level at peak no. Stress range (MPa) 4 1 96–10 = 86 6 5 80–10 = 70 2 3 47–15 = 32 8 7 35–15 = 20The damage resulting from each of these four stress ranges can now be calculatedin a tabular form as on the next page.
- 35. Fatigue-resistant Design 17.35 Stress range, ff (Mpa) Fatigue resistance (cycles) Damage due to 3.0 ¥ 106 loading cycles 86 6,273, 424a 0.478b 70 11,633,379 0.258 32 121,772,736 0.025 20 498,781,128 0.006 Total 0.767aUsing Eqn (17.6): log N = 12.601 – 3 log 86, N = 6,273,424 cyclesbUsing Eqn (17.17): ni /N = 3.0 ¥ 106/6,273,424 = 0.478Since the damage summation is only 0.767 (less than unity) the detail will be safeto take the stress history shown in Fig. 17.25 without fatigue failure.SummaryIn most practical situations, the type of loading will not be monotonic, i.e., it willnot increase steadily until failure occurs. Instead, the applied stresses fluctuate,often in a random way (Agerskov 2000). In some cases, the stress at a given pointon the surface varies cyclically from tension to compression and back again. In thepresence of cyclic stresses, it is found that premature failure occurs at stress levelsmuch lower than those required for failure under a steadily applied stress. Thisphenomenon of premature failure under fluctuating stress is known as fatigue andinvolves processes of slow crack growth. Components of buildings are not subjected to fatigue, but bridges, gantry girders,slender towers, offshore platforms, and structures supporting large rotatingequipment are prone to fatigue. Fatigue failures may be classified as high-cycleand low-cycle failures. Stresses associated with the low-cycle fatigue are generallyhigh and the fatigue life is described in terms of strain range (used in groundvehicle industries). Under high-cycle, low-stress fatigue, the material deformsprimarily elastically and the failure life is described in terms of stress range (as instructural applications). Fatigue crack initiation is mainly due to the effect of the stress concentration orflaw in the material. In welded steel structures, fatigue cracks start to grow fromthe imperfections or metallurgical discontinuities in the welds. The growth rate ofa crack is proportional to the square root of its length and, hence during the initiallife, the cracks are very small and hard to detect. Only in the last stages of life dothe cracks cause significant loss of cross section which leads to failure. Due tothis, it is very difficult to identify the crack growth in the initial stages, unless weuse non-destructive testing methods. The number of cycles of loadings, the stress range, and the type of memberdetail at the location are the three important parameters that affect the fatigue lifeof the component. Other factors that influence the fatigue behaviour are the stressconcentration, residual stress, plate thickness, imperfections, stress ratio, frequencyof cyclic loading, post-weld treatment, temperature, and environment. The presence
- 36. 17.36 Design of Steel Structuresor absence of non-metallic inclusions in the material also can have a significanteffect on the fatigue life. Fatigue strength is always checked under service-loadconditions. Though there are different approaches to fatigue analysis, stress method, usingS-N curves, is often used for structural applications. S-N curves show the relationshipbetween the number of cycles for fracture and the maximum stress range due tothe applied cyclic load. The fatigue strength of different welded details variesaccording to the severity of the stress concentration effect. In the code the mostcommonly used details are grouped into 15 main classes; also, the S-N curves areprovided for these 15 main classes. The data provided in these curves have beenobtained from a large amount of identical test specimens subjected to defined loadingconditions and measuring the number of cycles required for failure. S-N curves forshear stresses are also provided. A correction factor to take into effect the influenceof the thickness of the plate is also specified. The S-N curves given in most of the codes are for fully reverse load (R = –1)and zero mean stress. However, non-zero mean stress can also play an importantrole in fatigue design. In such cases the modified Goodman diagram is used. The fatigue life of components under variable-amplitude loading is calculatedusing the Palmgren–Miner rule, which is a linear damage rule. The two mainshortcomings of the linear damage rule (assuming sequence independence anddamage accumulation independence) can be overcome by non-linear damage rules.However, for structural applications, the Palmgren–Miner rule is found to givesatisfactory results. When the linear Palmgren–Miner rule is used, the variable-amplitude loading needs to be transformed into a series of constant-amplitudeloading. Out of the several methods available for cycle counting, reservoir countingand rainflow counting methods are explained with examples. Discussions on thefatigue assessment of hollow sections and guidelines for the fatigue-resistant designand detailing are provided. Fatigue cracking from out-of-plane effects and themethods to mitigate them are also discussed. An equation for the fatigue assessmentunder combined stresses is also given. The fatigue assessment procedure for steelstructures subjected to earthquake, based on deformation range (instead of thestress range of high-cycle fatigue curves), is also given based on research studies. Exercises 1. A crane girder of section ISMB 500 having a simply supported span of 8 m has to be checked for fatigue. The capacity of the crane is 300 kN and the gantry girder receives 75% of the total load as the reactive force. Assume that this force is applied as a single concentrated load. The crane operates 250 days/year and 6 hr/day. The crane makes a maximum of three trips per hour at this load level. Assuming the design life of the building to be 60 years, determine the fatigue assessment of this gantry girder.
- 37. Fatigue-resistant Design 17.37 2. After erecting the gantry girder in Exercise 1, it was decided to accommodate two more trips per hour at the same load level. Will the fatigue life of the gantry girder be still satisfactory? 3. Use the equivalent stress method to determine the percentage of life that has been expended by the loading applied to the gantry girder of Exercise 2. 4. The numerical values of peaks and valleys for the stress history of a gantry girder are shown below (see also Fig. 17.25) Peak/trough no Stress (in MPa) 1 93 2 18 3 55 4 8 5 85 6 10 7 37 8 18 Apply the reservoir counting method in order to identify the stress ranges in this stress spectrum and evaluate the effect of 3.5 ¥ 106 loading events of this stress history acting on a plate girder with multiple cover plates (category 37 of code). Review Questions 1. What is meant by fatigue and fatigue damage? 2. Why fatigue is not considered in the design of members in building frames? 3. Which structures are prone to fatigue failure? 4. Name the four stages of fatigue failure. 5. Explain the difference between high-cycle and low-cycle fatigue failures. 6. What are the two important factors that result in the initiation of fatigue cracks? 7. What flaws are there in rolled shapes? 8. How flaws may be introduced due to fabrication and erection? 9. Why most of the fatigue cracks may start from welds in a welded structure?10. Name some of the imperfections that are found in a weld.11. How are imperfections caused in a weld?12. Name the three important factors that affect fatigue life.13. What are the other factors that may influence the fatigue behaviour?14. Write short notes on the following factors which influence fatigue behaviour: (a) Stress concentration (b) Residual stress (c) Plate thickness (d) Imperfections (e) Stress ratio (f) Frequency of cyclic loading (g) Post-weld treatment
- 38. 17.38 Design of Steel Structures15. What are the three different approaches to fatigue analysis?16. Define stress range, mean stress, stress amplitude, and stress ratio.17. What is an S-N curve?18. Write the relationship between stress range and fatigue life as given in the code.19. Define fatigue limit and fatigue strength?20. What is the fatigue limit for normal steel members?21. What are the factors that affect the S-N curve?22. What are constant-amplitude fatigue limit and cut-off limit?23. What is the slope (m value) for fatigue strength curves used for shear stresses?24. State the conditions which when satisfied eliminate fatigue assessment.25. What are the partial safety factors for fatigue strength?26. State the equation which takes into account the influence of the thickness of plate.27. State the fatigue strength equations of a standard detail as given in the code for normal and shear stresses.28. How is the modified Goodman diagram constructed?29. State the Palmgren–Miner rule.30. What are the different methods used for cycle counting?31. Illustrate the procedure of cycle counting using the rainflow method.32. List some of the guidelines to be followed while designing and detailing welded joints for fatigue loads?33. How can we arrest and repair a fatigue crack emanating from out-of-plane effects?34. Why are coped ends of beams susceptible to fatigue cracking?35. State the equations (Miner’s summation) to take into account combined stresses?

No public clipboards found for this slide

×
### Save the most important slides with Clipping

Clipping is a handy way to collect and organize the most important slides from a presentation. You can keep your great finds in clipboards organized around topics.

Be the first to comment